1. International Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 3189||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||A Study of Influence of Electrochemical Process Parameters onthe Material Removal Rate and Surface Roughness of SS AISI3041,S. S. Uttarwar, 2,Dr. I. K. Chopde1,Department of Mechanical Engineering, Priyadarshini College of Engineering, Nagpur, Maharashtra, India2,Department of Mechanical Engineering, Visvesvaraya National Institute of Technology, NagpurMaharashtra, IndiaAbstractThe machining of complex shaped designs was difficult earlier, but with the advent of the newmachining processes incorporating in it chemical, electrical & mechanical processes, manufacturing hasredefined itself. This paper presents results of the Electrochemical Machining (ECM) process, which was usedto machine the SS AISI 304. Specifically, the Material Removal Rate (MRR) and Surface Roughness (SR) as afunction of ECM were determined. The experimental work was based on the Taguchi approach ofexperimentation and table L32 was used. Furthermore, a theoretical and computational model is presented toillustrate the influence parameter variations in results. The influence of independent parameters such as time ofelectrolysis, voltage, current, concentration of electrolyte, feed rate and pressure on output parameters materialremoval rate and SR is studied in this work. The results indicated that MRR was remarkably affected byvariation in current and Surface Roughness decreased with increase in current. Hence, it was apparent thatirregular MRR was more likely to occur at high currents. The results showed that MRR increased withincreasing electrical voltage, molar concentration of electrolyte, time of electrolysis and feed rate. However, thetime of electrolysis was the most influential parameter on the produced surface finish.Keywords: Electrochemical machining; Material removal rate; Time; Feed rate; electrolyte concentration,Anova, Percentage error.1. IntroductionElectrochemical machining (ECM), a nontraditional process for machining[1,2]has been recognizednow a days for performing numerous machining operations.[4]Earlier the machining of complex shaped designswas difficult, however, with the advent of the new machining processes that incorporate in it chemical, electricaland mechanical processes, manufacturing process has redefined itself.[3]New materials which have highstrength to weight ratio, heat resistance, hardness and are also complex shapes needing greater accuracy demanddevelopment of newer type of machining process. The new and improved machining processes are oftenreferred to as unconventional machining processes. For e.g. ECM removes material without heat. Almost alltypes of metals can be machined by this process. In today‟s high precision and time sensitive scenario, ECM haswide scope for applications.[5]More specifically, ECM is a process based on the controlled anodic dissolution ofthe work piece anode,[6]with the tool as the cathode, in an electrolytic solution.[11]The electrolyte flows betweenthe electrodes and carries away the dissolved metal.Since the first introduction of ECM in 1929 by Gusseff, its industrial applications have been extendedto electrochemical drilling, electrochemical deburring, electrochemical grinding and electrochemicalpolishing.[13]More specifically, ECM was found more advantageous for high-strength alloys. Today, ECM hasbeen increasingly recognized for its potential for machining,[7]while the precision of the machined profile is aconcern of its application.[9,10]During the ECM process, electrical current passes through an electrolyte solutionbetween a cathode tool and an anode work piece.The work piece is eroded in accordance with Faraday‟s law of electrolysis.[12]ECM processes findwide applicability in areas such as aerospace and electronic industries for shaping and finishing operations of avariety of parts that are a few microns in diameter.[13]Furthermore, it has been reported that the accuracy ofmachining can be improved by the use of pulsed electrical current and controlling various process parameters.Amongst the often considered parameters are electrolyte concentration, voltage, current and inter electrodegap.[14]Though there is a possibility of improving the precision of work, the dependency of accuracy onnumerous parameters demand that a thorough investigation should be carried out to ascertain the causality todifferent parameters. In the backdrop of above information, this study was carried out to assess the bestconditions (with respect to different process parameters) for improving the accuracy of ECM process. In thispaper the authors propose an analytical model of electrochemical erosion to predict the finishing machined work
2. A Study Of Influence Of Electrochemical Process Parameters…190||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||piece. The study envisaged an empirical data obtained from the experiments carried out to assess effect ofoperating parameter variations on material removal rate (MRR) and surface roughness (SR) for Stainless steel(AISI 202).2. ECM SetupFig 1and 2 shows the schematic set up of ECM in which two electrodes were placed at a distance ofabout 0.1 to 1mm and immersed in an electrolyte, which was a solution of sodium chloride.[15]When anelectrical potential (of about 20V) is applied between the electrodes, the ions existing in the electrolyte migratetoward the electrodes[15].Fig 1. ECM SetupFig 2. Block diagram of ECM setup3. ECM Process Characteristics3.1 Material removal rate:The MRR primarily depends on the feed rates. The feed rate determines the amount of current that canpass through the work and the tool. As the tool approaches the work piece the length of the conductive currentpath decreases and the magnitude of current increases. This continues until the current is just sufficient toremove the metal at a rate corresponding to the rate of tool advance. Thereafter a stable cut is made availablewith a fixed spacing between the work and the tool, which is termed as the equilibrium-machining gap. If thetool feed rate is reduced, the tool advance will momentarily lag behind, increasing the gap and thus resulting in areduction of current. This happens until a stable gap is once again established. Thus, the feed rate is animportant parameter, which was given due consideration in the experiment.3.2 AccuracyUnder ideal conditions and with properly designed tooling, ECM is capable of holding tolerance of theorder of .02 mm & less. Repeatability of the ECM process is also very good. This is largely due to the fact thatthe tool wear is virtually non-existent on a good machine; tolerance can be maintained on a production basis inthe region of .02-.04 mm. As a general rule, the more complex the shape of the work, the more difficult is tohold tight tolerances and the greater is the attention required for developing a proper tooling and electrodeshape.3.3 Surface FinishECM under certain conditions can produce surface finishes of the order of 0.4mm. This can beobtained by the frontal cut or the rotation of the tool or the work. Hence care was taken to control the importantvariables affecting the surface finish are feed rate, voltage, electrolyte composition, pressure, current & flow.
3. A Study Of Influence Of Electrochemical Process Parameters…191||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||4. Operating Parameters In ECMThe operating parameters which are within the control of the operator and which influence ECMprocess capabilities are as follows: [14],[15]4.1 VoltageThe nature of applied power supply is of two types, DC (full wave rectified) and pulse DC. A full waverectified DC supplies continuous voltage and a pulse generator is used to supply pulses of voltage with specificon-time and off-time. The MRR is proportional to the applied voltage. But, the experimental values were foundto be varying non-linearly with voltage. This is mainly because of less dissolution efficiency in the low voltagezone as compared to the high voltage zone.[12]However continuous voltage supply is used for thisexperimentation work.4.2 Feed RateFeed rate governs the gap between the tool (cathode) and the work piece (anode) it is important formetal removal in ECM.[6]It plays a major role for accuracy in shape generation and hence was constantlymonitored.4.3 Electrolyte and its concentrationECM electrolyte is generally classified into two categories, passivity electrolyte containing oxidizinganions e.g. sodium nitrate and sodium chlorate, etc. and non-passivity electrolyte containing relativelyaggressive anions such as sodium chloride. Passivity electrolytes are known to give better machining precision.This is due to their ability to form oxide films and evolve oxygen in the stray current region. From review ofpast research, in most of the investigations researchers recommended NaClO3, NaNO3, and NaCl solution withdifferent concentration for ECM and hence, NaCl was used as an electrolyte in this experimentation withconcentration of 125gm/lit and 150gm/lt.4.4 CurrentCurrent plays a vital role in ECM. The MRR is directly proportions to the current (i.e. MRR increaseswith increase in current). However, this increase can be observed up to a certain limit and exceeding currentbeyond this level negatively affects accuracy and finishing of work piece. Hence, care was taken to applycurrent in the desired way.5. Experimental SetupFig 3 shows actual photograph of the experimental set up of ECM on which the experimentationprocess was carried out.Fig 3. Experimental set up of ECM process5.1 Tool and Work piece MaterialThe tool used in this study was made up of copper while the work-piece used is this study was made upof Stainless Steel SS 304. This work piece was selected for this study as it has wide applications in variousfields. The chemical composition of the used work piece i.e. SS 304 are as followsSample C(%)Si(%)Mn(%)P(%)S(%)Cr(%)Ni(%)Cu(%)Fe (%)SS 202 0.023 0.447 1.16 0.038 0.016 18.31 7.99 1.05 Remaining
4. A Study Of Influence Of Electrochemical Process Parameters…192||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||Fig 4. Chemical characteristics of work piece SS 3045.2 Experimentation WorkAn Orthogonal Array L32(21*45) of Taguchi method was used for conducting the experimentationwork. The results of dependent parameters (MRR and SR) with respect to all levels of independent parametersare shown in a following table.Table 2 Values of Dependent and Independent Parameters (Orthogonal array L 32)RunNo.Independent parameters Dependent parametersElectrolyteConc.(gms/Ltr)Voltage(V)Current(Amp)Feed(MM/min)ElectrolyteFlow(Ltrs/min)Pressure(Kg/Cm2)MRR(mg/min)SR(µm)E B A 0.1 C F G H1125 10 100 0.2 4 3.45.277 4.0742125 10 125 0.3 5 3.65.224 3.7883125 10 150 0.4 6 3.75.259 3.7754125 10 175 0.1 7 3.86.380 5.5915125 14 100 0.2 5 3.64.430 3.6266125 14 125 0.3 4 3.45.586 3.3067125 14 150 0.4 7 3.85.161 3.4918125 14 175 0.2 6 3.74.136 3.3049125 18 100 0.1 6 3.84.705 3.67710125 18 125 0.4 7 3.75.859 3.60311125 18 150 0.3 4 3.66.056 5.09912125 18 175 0.2 5 3.44.811 4.47413125 22 100 0.1 7 3.74.497 4.01314125 22 125 0.4 6 3.85.365 3.57315125 22 150 0.3 5 3.45.086 3.76016125 22 175 0.4 4 3.64.789 3.45817150 10 100 0.3 4 3.85.612 4.299
5. A Study Of Influence Of Electrochemical Process Parameters…193||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||18150 10 125 0.2 5 3.74.922 3.36219150 10 150 0.1 6 3.65.373 3.51020150 10 175 0.4 7 3.45.343 3.25921150 14 100 0.3 5 3.76.703 6.40222150 14 125 0.2 4 3,84.514 3.26823150 14 150 0.1 7 3.46.705 5.97124150 14 175 0.3 6 3.65.468 3.71325150 18 100 0.4 6 3.45.144 3.14926150 18 125 0.1 7 3.64.657 3.60227150 18 150 0.2 4 3.75.439 4.61228150 18 175 0.3 5 3.86.754 4.47429150 22 100 0.4 7 3.64.772 3.94730150 22 125 0.1 6 3.44.540 3.53031150 22 150 0.2 5 3.85.362 3.58932150 22 175 0.3 4 3.73.607 3.270∑4400 512 4400 0.4 176 112.2165.044 124.5665.3 Mathematical Model for MRR and SRUsing Regression Analysis Mathematical models were developed for MRR and SR with their indices.The six decision variables concerned for this model were Current, Voltage, feed rate, Pressure, Electrolyteconcentration and flow of electrolyte.6. ObjectivesThe various objectives under consideration for the formulation of model werea) Maximization of MRR andb) Improving SR (surface finish) and dimensional accuracy6.1 Derived mathematical ModelsEquation 1 and 2 are the mathematical models derived for calculation of MRR and SR.MRR = Constant × Aa× Bb× Cc× Dd× Ee× FfWhere a,b,c,d,e,f are the indices for current, voltage, electrolyte flow, feed rate, Electrolyte concentration andpressure . The formulated models are as followsMathematical Eqn for MRR isMRR= 3.14695 A0.002050* B-0.01061875*C0.001225*D0.10975*E- 0.00345*F-0.0104625--- Eqn 1Mathematical Eqn for SR isSR= 2. 2425000 A0.0024500* B-0.0196875*C0.0212500*D0.0375000* E- 0.0022500*F0.0093750-----------Eqn 2From the Eqns. 1 and 2, it was evident that the MRR was positively influenced by the independentvariables such as current, electrolyte flow and feed rate whereas negatively influenced by voltage, electrolyteconcentration and pressure. Moreover, the SR was observed to be positively influenced by current, electrolyteflow, feed rate, and electrolyte concentration whereas it (SR) is negatively influenced by voltage and electrolyteconcentration.7. Comparison Of Practical V/S Theoretical Values Of MRRA sample set of Comparison of Actual value of MRR calculated by formula and corresponding valuesderived by mathematical model is shown in Table 3 along with the calculated percentage error.
6. A Study Of Influence Of Electrochemical Process Parameters…194||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||Table 3: Comparative assessment of the Practical v/s Theoretical values of MRRSr. No.Values of Dependent Parameter (MRR) PercentageErrorBy Mathematical Model Actual Experimentation15.591386235 5.277 5.957724.994041391 5.224 -4.402034.671671187 5.259 -11.168144.458360504 6.380 -30.119755.636831741 4.430 27.242364.987908572 5.586 -10.70707.1 Comparison of Practical v/s Theoretical values of SRA sample set of Comparison of Actual value of SR calculated by formula and corresponding valuesderived by mathematical model is shown in Table 4 with Percentage error.Table 4: Comparative assessment of the Practical v/s Theoretical values of SRSr. No.Values of Dependent Parameter (SR) PercentageErrorBy Mathematical Model Actual Experimentation13.367250843 4.074 -17.347823.374170425 3.788 8.850133.384412557 3.775 -10.346745.2312324 5.591 -6.434853.368413193 3.626 -7.103963.350383833 3.306 1.34258. Percentage ErrorPercentage error graphs for difference in actual and theoretical values of MRR and SR are plotted witherror on Y axis and readings on X axis. Fig 5 and 6 shows percentage error in actual and experimental values ofMRR and SR. It was evident from the graphs that the different test runs showed noticeable variation in thepercentage error of both the dependent parameters i.e. MRR and SR.Fig 5. Percentage Error Graph for MRR
7. A Study Of Influence Of Electrochemical Process Parameters…195||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||Fig 6. Percentage Error Graph for SR9. Analysis of Variance or ANOVAAnalysis of Variance or ANOVA is a general technique that can be used to test the hypothesis that themeans among two or more groups are equal, under the assumption that the sampled populations are normallydistributed. The ANOVA procedure was used to test hypotheses that several means are same. In this study atotal of 32 different conditions were selected to study the Material Removal Rate and Surface Roughness. Thepreliminary comparative assessment was carried out using the ANOVA procedure, followed by Post Hoc Test.The Post Hoc Test was employed to check, which means (obtained from the MRR and SR values as a functionof 32 different runs. In addition to this, the Tukey‟s HSD test was also performed to determine the HSD i.e.Honestly Significant Difference.Anova and Post Hock TestSS304N MeanStd.DeviationStd.Error95% Confidence Intervalfor MeanMinimum MaximumLowerBoundUpperBound1 3 3 5.2540 .09115 .05262 5.0276 5.4804 5.162 3 3 5.3193 .19453 .11231 4.8361 5.8026 5.12ANOVA Results for MRRSum ofSquares df Mean Square F Significance.SS 304 BetweenGroups50.491 31 1.629 29.513 .000WithinGroups3.532 64 .055Total 54.023 95ANOVA Results for SRSum ofSquares dfMeanSquare F Sig.SS 304 BetweenGroups74.024 31 2.388 18.957 .000WithinGroups8.062 64 .126Total 82.086 95
8. A Study Of Influence Of Electrochemical Process Parameters…196||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||10. ResultsIt was observed that MRR was considerably affected by variation in current and SR decreased withincrease in current. Hence, it was apparent that irregular removal of material was more likely to occur at highcurrents. The NaCl electrolyte was responsible for the lower SR and over-cut. Furthermore, MRR increasedwith flow rate because there was more mobility of the ions from the metal to the solution, thereby increasing thespeed of the chemical reactions. Besides, there was a need to constantly remove the sludge formed duringmachining, which was necessary as the sludge accumulation could have negatively affected the machiningefficiency of the ECM process. Results of entire experimentation work are as under:A) Optimum value of MRR is as followsActual By ModelOptimum Value of MRR 6.754 mg/min 5.654 mg/minCorresponding value of SR for this MRR 3.5574 µm 3.375 µmValues of various parameters for above said maximum value of MRR is Current- 175A,Voltage 18 volts, FlowRate 5Ltr/Min, Feed 0.3mm/min, Electrolyte concentration 150g/lit, Pressure 3.8 kg/cm2B) Optimum value of SR is as followsC)Actual By ModelOptimum Value of SR 3.259 µm 3.46560 µmCorresponding value of MRR for this SR 5.343mg/min 5.7883mg/minValues of various parameters for above said optimum value of SR is Current- 125A, Voltage-10 volt, FlowRate -7Ltr/Min, feed-0.4mm/min, Electrolyte concentration 150g/Lit, Pressure 3.4 kg/cm2The mean MRR for SS304 varied between 3.6070 and 6.7540. Lowest MRR was observed for the run no. 32,while the highest value was recorded for the run no. 28. The analysis of data following ANOVA indicatedsignificant difference in the mean values MRR and SR as a function of different conditions (set for differentruns).11. ConclusionThe experimentation work consists of study the influence of process parameters on MRR and SR.Process parameter such as machining voltage, feed, Current, Electrolyte concentration, electrolyte flow weresuccessfully controlled and were allowed to vary according to need. The different combinations of thecontrolling factors were considered for the experimentation and to determine their (independent parameter‟s)influence on MRR and SR of SS304 work piece. The experimentation was carried out by varying all parametersin combination as per orthogonal array L32. On the basis of the results obtained in this work, main conclusioncan be stated as the selection of appropriate values for the different parameters of ECM process is crucial toachieve the efficiency and high quality of outcome from the process. Furthermore, similar experimental workcan be continued to determine optimum process conditions for ECM process for other metals. In addition to thisthe difference between the theoretical and practical values of MRR and SR are also required (for other metals)to give some thought, so that % error can be reduced.References[1] J.A. Mc Geough, Principle of Electrochemical Machining. Chapman and Hall, London, 1974.[2] P. Asokan, R Ravikumar, R Jeyapaul, M Santhi “ Development of multi objective optimization modelsfor Electrochemical Machining Process” Springer. Int J Adv. Munaf Technol( 2008) 39:55-63 DOI10.1007/s00170-007-1204-8[3] M. Haıdopoulos · S. Turgeon · C. Sarra-Bournet · G. Laroche · D. Mantovani “Development of anoptimized electrochemical process for subsequent coating of 316 stainless steel for stent applications”Received: 19 January 2004 / Accepted: 24 October 2005 Springer Science+Business Media, LLC 2006
9. A Study Of Influence Of Electrochemical Process Parameters…197||Issn||2250-3005|| (Online) ||March||2013|| ||www.ijceronline.com||[4] K.L. Senthil Kumar, R. Sivasubramanian, K. Kalaiselvan, “Selection of Optimum Parameters in NonConventional Machining of Metal Matrix Composite” Portugalia Electrochemica Acta 2009 27(4) 477-486.[5] R V Rao, P J Pawar, R Shankar “Multi objective optimization of electrochemical machining processparameters using a particle swarm optimization algorithm” DOI:10.1243/09544054JEM1158 Proc. Imech E Vol 222 (2008) Part B[6] J.A. McGeough and X. K. Chen, Machining methods: electrochemical, in “Kirk-Othmer J. I.[7] S K Mukherjee, s Kumar, P K shrivastava, Arbind Kumar “ Effect of valency on material removal ratein electrochemical machining of aluminium” Elesevier Journal of material processing Technology202(2008) 398-401[8] B Bhattacharyya S K Sorkhel “ Investigation for controlled electrochemical machining throughresponse surface methodology based approach”Elesevier Journal of Processing Technology 86(1999)200-207.[9] Jo˜ao Cirilo da Silva Neto, Evaldo Malaquias da Silva, Marcio Bacci da Silva, „Intervening variables inelectrochemical machining‟ Journal of Materials Processing Technology 179 (2006) 92–96[10] J.A. McGeough, Advanced Methods of Machining, Chapman and Hall, London, 1988, pp. 55–88.[11] J. Tlusty, Manufacturing Process and Equipment, 1st ed., Prentice-Hall, USA, 2000.[12] M. Datta, Anodic dissolution of metals at high rates, IBM J. Res. Develop.37 (2) (1993) 207–226.[13] M. Datta, R. V. Shenoy, L. T. Romankiw, “Recent advances in the study of electrochemicalmicromachining,” ASME J. Eng. Ind. 118, 29–36, 1996.[14] P.C. Pandey, H.S. e Shan, Modern Machining Processes, Tata McGraw Hill, New Delhi, 1980.[15] G.F. Benedict, Nontraditional Manufacturing Processes- Electrochemical Machining, Marcel Dekker,New York and Basel, 1987, pp. 125–172.
Be the first to comment